Journal of the Korean Physical 80ciety(Proc. 8uppl.), Vol. 28, December 1995, pp. 8609-8616

Building a Better World with Buckyballs David TOMANEK Department of Phy&ic& and A.dronomy and Center for Fundamental Materials RC8eorch Michigan State Univcrsity, Ecut Lan8'ng, Michigan 48894-1116, U. S. A.

The 0 60

"buckyball" a prominent member of the recently discovered family of fullerene molecules, I

is an unusual system with exciting properties. This contribution summarizes the present state of theoretical understanding of the equilibrium structure of carbon clusters, in particular the fullerenes,

the optical properties of individual fullerene molecules, superconductivity in the alkali-intercalated Ceo solid, and the disintegration of fullerenes in collisions and at high temperatures.

I. INTRODUCTION Until very recently, the only stable bulk forms of elemental carbon have been believed to be graphite and diamond. About ten years ago, this conventional wisdom has been challenged by the discovery of the stable C60 molecule with a spherical hollow cage [1]. This molecule, .tKJmetimes called "buckyball", turned out to be only a particular representative of the family of ''fullerene" molecules, named so for their close resembla.ncc to the geodesic dome structures created by the architect Buckminster Fuller. Later on, it has been found that Cso molecules can aggregate to form a molecular crystal. The interest in C60 rose dramatically following the successful development of a mass production technique for this system [2]. The resulting research first concentrated on characterizing this molecule and the corresponding solid. Next, spurred by the discovery of superconductivity in the alkali intercalated C so solid [3,4], substantial effort has been invested in modifying the C 60 molecule and solid, and in the synthesis of other fullerenes. Ongoing research focuses both on the structural and electronic properties of C60inspired carbon fullerenes. At present, most emphasis is pla 20, we find rings to be more favorable than chains, since releasing the dangling bond energy of a chain easily offsets the bending energy when forming a ring. At these 181'ger ai~es, however, higher coordinated structures turn out to be energetically much more favorable. For n > 20, we find the hollow fullerenes to be the most stable isomers. Alec in this size range, the average binding energy per atom is gradually increasing with in-

creasing fullerene size, approaching the value found in a graphene sheet [15]. At sizes exceeding 700 atoms, finally, multi-walled structures are found to be most stable, due to the significance of the attractive interaction between adjacent walla [15]. The Coo does not appear to be exceptionally stable. Since in thermodynamic equilibrium the relative abundance of different cluaters should reflect their stability, our

0.7 ~

:> OJ

~

'" 0 0

i'il

6.6

...... ' ...

6.5

.x'

,"

~..

" .•.•.•.••........ •...... "/.:.~.,, .....

6.4 6.3 6.2

6.1 6. a

.........

"

,

..jIIl

"

••-"'..~_...L'_-'-_L-~_--'-_--'-..--.J

~

~

~

M

~

~

50

9

60

n

Fig. 1. Binding energy per atom E coo in small carbon eluate... as a function of eluster size n, (a) for n ~ 20 and (b) for n ~ 20. R..aults for cbains (0) are connected by a solid line, results for ~ (0) are connected by a dashed line, and results for planar grapbite flakes (.) are connected by a dotted line. Results for buckled fullerene caps with a pentagonal ( x) or a hexagonal baais (+) are connected by a dashed line. Results for hollow fullerene cages (.) are connected by a solid line. (From Ref. [9], @American Physical Society.)

results would suggest a continuous size distribution of carbon fullerenes in the mass spectra. This is in clear con-

2. Collective electronic excitations in Ceo clusters

trast with the observed abundance of the 60-atom struc-

The structural similarity between a Coo molecule and graphite raises the question, whether the optical response of this finite system may have any resemblance with that of macrOBCopic graphite. In the following, I willleview resulta for the dynamical dipole response of flee Coo me>-

ture. We must conclude that simulations beyond these T '" 0 stability considerations are nece..ary to explain

the abundance of the "magic" Coo cluster in the m.... spectra.

Journal of the Korean Physical Society(Proc. SuppI.), Vol. 28, December 1995

-8612-

leeules, published previously in Ref. [16], with emphasis on the discussion of collective plasmon-like excitations. The optical response of clusters to an external field is described within linear response using the Random Phase Approximation (RPA) [17]. In the present case, the single-particle spectrum is obtained using the parametrized LCAO Hamiltonian discussed previously. The occupied states spread over 19.1 eV, in good agreement with the publisbed LOA value of 18.8 eV [18J. The calculated gap between the highest occupied molecular orbital (HOMO) and the lowest unoccupied molecular orbital (LUMO) is 2.2 eV, larger than the 1.8 eV value which is underestimated in LDA [18]. The "1r" states near the HOMO-LUMO gap, and the more strongly bound "IT" states have a similar character as the corresponding states in graphite. The icosahedral symmetry of Cso allows us to distinguish singly-, triply-, quadruply- and pentuply-degenerate levels. A large number of optical transitions is allowed by the dipole selection rules. In the particular case of a dynamical dipole field along the z-direction, which is applied to a spherical molecule such as Cs o, the calculation can be simplified significantly by anticipating the form of the dipole operator which describes the response of the system. As discussed in Ref. [9], the dipole operator D, is dominated by two contributions:

Dl1)

J

origina.ting in the intersite charge trans--

fer across the molecule, and D}2) , stemming from the polarization of individual carbon atoms. In the free response, which ignores the screening of transitions by electron-hole pair excita.tions, the lowest dipole-allowed tr8Illlition is the IIOMO - t LU MO + I transition which occurs at an energy 1u..J < 3 eV. In the RPA treatment of dynamical screening, the low-lying transitions are slightly blue shifted and, more important, their oscillator strength is reduced by a factor of typically 10 with respect to the free response. A factor of 400 quenches the HOMO - t LU MO + I transition to only an insignificant peak in the spectrum. Even though the calculated spectrum in the frequency range rn" < 10 eV resembles the observed absorption spectrum in a dilute Cso solution [19), the integrated oscillator strength in this range remains well below the value of 240 (which is the total number of active electrons), as predicted by the fsum rnle. The missing oscillator strength is fOWld at higher energies. The oscillator strength, which occurs as a dense featureless spectrum in the free response, piles up to a giant collective excitation at rn" "" 30 eV in the RPA response calculated with ill') only. The consideration of also Dlztinduced transitions causes a fragmentation and red shift of this mode into an energy range of rn" "" 20 eV. This prediction has been subsequently confirmed by the observation of a giant resonance at rn" '" 20 eV in the photoionization spectrnm of CGO [20]. Collective excitations at frequencies ranging between 20 - 30 eV have also been observed in Cso films [21-23). To investigate the nature of this collective mode, an

LOA-RPA calculation was performed for an infinitely thin spherical jellium shell with the radius of Cso, carrying 240 conduction electrons [16]. The calculation predicted a single absorption peak at a frequency &.1,,;15 - 20 eV, which lies very close to the Mie plasmon frequency rn"Mi, = h[41rpe 2/(3m»)'/2 ",25 eV of a solid metal sphere with 240 free electrons and the radius of the Cs o cluster. The origin of the high value of the collective mode frequency is consequently the large valence electron density p in the CGO molecule. This leads to the conclusion that collective electronic excitations occur in fullerenes as small as tbe C so molecule. The nature of these modes, which occur at frequencies far beyond the HOMO-LUMO gap, resembles closely that of a classical Mie plasmon. A more refined calculation of the RPA response of fullerenes to external fields [24], not restricted to the dipole response described by D}') and Di2 ) , shows that the excitation spectrum of probably all fullerenes (investigated were C,o, C so and 070) is dominated by the above discussed "(1" mode at hw.,.R::20 eV and a softer "1f'" mode at rn"."'6 eV. These two modes have also been observed in electron energy loss spectra of Cs o fullerite films [23], and appear to be the analogues of the 1r and IT plasmons in graphite [25]. In graphite, the low-frequency 1r mode has been interpreted by the in-plane response of the weakly bound P. system to a field parallel to the layers. The high-frequency IT mode has been assigned to the out-ofplane motion of the strongly bound IT system of 8 and P electrons in response to a field perpendicular to the layel'S.

It appears that the finite fullerene molecules show a well-defined signature of plasmon modes which are closely related - in nature and in frequency - to the IT- and 1rplasmons of graphite. The large oscillator strength of these modes is collected from lower-lying particle-hole excitations which consequently experience strong dynamical screening.

3. Superconductivity in the alkali doped CGO solid Potentially the most important property of the C so solid is its superconducting behavior when doped with alkali atoms [3,4). In the following, I will present a quantitative Bardeen-Cooper-8chrieffer (BC8) theory which has been used successfully to describe the superconducting behavior of Cso [26]. The electronic states of the alkali doped M,C GO solid are calculated using the LOA and the LCAO formalism discussed above. The vibr.... tional modes of the solid are determined using an extended Keating Hamiltonian which describes both on-ball and inter-ball vibrations. McMillan's expression for the critical temperature for superconductivity Tc reads [27] Tc

_ rn,,'og -

(-1.04(1+ .\) ) 1.2 kB ezp .A - ,,- _ 0.62.\,,-

(9)

Building a Better World with Buckyballs - David TOMANEK In accordance with other standard superconductors, 1" "" 0.1 was used for the effective Coulomb repulsion. The stiff on-ball vibrational modes of Coo yield .~' •• "" 1400 K for the "Debye temperature" of the solid. ir.'th the electronphonon coupling constant A "" 0.6, to be derived below, we can explain the observed value T, "" 30 K in Rb3 C. O

[4]. The electron-phonon coupling constant is given by A = 2N(Ep )V, where N(E p ) is the electronic density of states at the Fermi level, and Y is the Bardeen-Pines interaction which couples two electrons to a Cooper pair. The large value of A is a consequence of both a large density of states at the Fermi level and a strong coupling of these states to vibrational states. The conduction band is derived from the lowest unoccupied molecular orbital (LUMO) of C. O, and has P. character. Due to the small inter-ball hopping, the width of this band is small, W""0.5 eV [18,28J. For a featureless (e.g. rectangular) band, one can estimate N(Ep ) "" 6/0.5 ey-l .. 10 ey-l. LDA calculations give N(Ep ) "" 20 ey- 1 for a half filled band [18,28]. This density of states is at least one order of magnitude larger than that of intercalated graphite, consistent with the finding that T,(intercalated graphite) «Tc(M3Cso), The vibrational eigenmodes of the crystal were determined using an extended Keating Hamiltonian, with parameters adjusted to reproduce the vibrational spectra of the C.O solid. The coupling to the conduction states was investigated for each of these modes. These calculations showed that coupling of the librational modes at v "" 10 em-I can be neglected, while inter-ball optical modes at v .. 100 em-I couple weakly. The important modes are on-ball modes at a frequency range v "" 200 - 1600 em-I. Among the most strongly coupling modes are the radial buckling H. modes at v" 400 em -1, the tangential pentagon breathing A. mode at v "" 1600 em-I. and tangential optical H. modes at V"" 1600 em-I. These modes gave a value of V",,21 meV per Cso. The above determined large values of V and of N(E p ) are responsible for a large electronphonon coupling constant A. The dominant contribution of on-ball modes to the electron-phonon coupling makes it possible to treat electron-phonon coupling in relationship to a dynamical Jahn-Teller effect for the charged C. o molecule, and consider solid Cso as a molecular crystal [29]. In this case, when changing the alkali intercalant M in M3CSO, Aand consequently also T, should only depend on the Cso-C.o separation which modifies N (EF). One would expect an increase of T" with increasing lattice constant of M3C.o, which is achieved by substituting a heavier alkali element M [28]. The same argument would lead to the conclusion that a reduction of the lattice constant, due to increasing pressure, should result in a reduction of T,. Both these effects have been verified experimentally [28]. In conclusion, standard BCS theory was found to be capable of providing a quantitative explanation of super-

I,.

-5613-

conductivity in the alkali doped Cso solid. The observed large value of T, is linked to the high Debye temperature, a large value of N(E p ), and a strong coupling of on-ball vibrational modes to states at Ep [26,28]. 4.

Collision dynamics of fullerenes

Next, I will discuss the stability and reactivity of C n fullerene clusters in binary collisions. Of particular interest in this study was the question of a potential synthesis of more complex structures, such as multi-walled fullerenes (or "bucky onions") [5], by impact-induced encapsulation of the smaller C. o buckyball inside the larger C240 fullerene. In order to better understand the reaction dynamics, the motion of the individual atoms during the collision process was visualized in

& video

movie.

Microcanonical molecular dynamics simulations of the collision process were performed at different initial center-of-m.... kinetic energies. The Cso and the C240 clusters were prepared in their equilibrium structures. In the first set of simulati()ns investigating central collisions, the clusters were given an initial linear momentwn, zero angular momentum, and the impact parameter was set to zero.

At a low 10 eV center-of-m.... kinetic energy, the collision between the C240 and the C.o clusters could be best characterized as an elastic recoil. At a ten times higher center-of-mass energy of 100 eV, the C,.o-C. o collision is best described as quasielastic scattering. At the point of impact of C.O onto the C 24 0 cluster, one can observe a heat- and shock-wave propagating fast within the structure, starting at the point of contact. The C,.o-C. o agglomerate is capable of storing the large surplus energy in a substantial structural deformation and the many vibrational degrees of freedom of the system. In spite of the extreme deformations which even result in a negative Gaussian curvature of the

C240

cluster, both clusters depart intact, without exchanging any atoms. Finally, at only three times higher center-of-m.... energy of 300 eV, the C,.o-C.o collision leads to an impactinduced fragmentation. The intuitive expectation, that the more rigid C60 structure might penetrate the "floppy" wall of the larger C240 fullerene, proves to be incorrect. The opposite process occurs - it is the smaller C60 cluster which fragments first, leaving the larger C240 structure vibrationally highly excited, yet intact. Cso is observed to fragment into a structure consisting of linked chains and rings, as well as fragments. A very similar fragmentation dynamics is also observed in simulations asswning

&

nonzero impact parameter and nonzero ini-

tial angular momentum of the fullerenes prior to collision. The physics underlying this particular fragmentation process is relatively simple. Upon impact, the exces&ive center-of-mass kinetic energy is distributed into the internal degrees of freedom of both clusters; this vibra-

-8614-

Journal of the Korean Physical Society(Pmc. Suppl.), Vol. 28, December 1995

(a) Solid phase

(b) Floppy phase

(e) Pretzel phase

T=1000

T=3000 K

T=4200 K

(d) Linked chains

(f) Chain gas

T=5000 K

T=10200 K

cf)

Fig. 2. llSnap shots" illustrating the geometry of a 060 dU8teT at temperatures COI'1"'""Ip'l to the different "phases"

dillCWlOed in the text. (From Ref. [30], @American Physical Society.) tional energy appears as heat. The fewer degrees of freedom of the smaller C.o cluster experience a higher excitation which results in a higher temperature. Due to the limited amount of vibrational energy which can be stored in the anharmonic potentials, the energy surplus is consumed in the heat of "melting" and partly the heat of "evaporation". The structural transformation of the fragmented Ceo cluster at high temperatures is driven by the vibrational and structural entropy which is obviously much higher for the floppy one-dimensional chain and ring substructures than the more rigid fullerene structure. If this explanation is correct~ the same structure con~ sisting of linked rings and chains should also occur in isolated fullerenes which have been exposed to temperatures beyond those causing melting. AJ, will be shown in the following Subsection, this is indeed the case. More important, this establishes an intriguing link between the impact- and thermally-induced fragmentation of clusters.

Ii.

How do buckyballs melt?

The present study, originally inspired by the surprising results of above described inelastic collisions, is intended to answer some fundamental questions related to the nature of thermally induced structural transformations in fullerenes and finite clusters in general. The first important question is, whether atomic clusters - such as fullerenes - undergo "phase transitions" such as melting, and what the "phase diagram" would look like. Next, one would like to know how to best characterize the.. "phases". Finally, one would like to understand the drivang force for such "phase transitions" . These and some other related questions have been addressed in a Nose-Hoover molecular dynamics simula.tion of the melting and evaporation process of three prototype fullerenes, namely C20, Coo, and C 240 . The detaila of the simulation are discussed in Ref. [30]. The reBults

Building a Better World with Buckyballa - David TOMANEK

-S615-

presented below complement nicely those of recent microcanonical ensemble simulations on C 60 and C70 [31]. The key result of the simulation is the total energy of an iaolated fullerene as a function of heat hath temperature. In the temperature range of interest, namely between 1,000 K and 10,000 K, the energy E shows a generally linear increase with temperature. The specific heat cv = dE/ dT is generally close to the classical value cv = 3kB/particle. Strong peaks in the specific heat occur close to 3,000 K and 4,000 K. The peaks get more pronounced with increasing size of the system and, since

higher temperatures, the spectrum broadens and the average stability of the structure decreases. A simple estimate of the "melting transition" from fullerenes to pretzels can be obtained by comparing the free energies of the two structures which must be equal at the melting point. At this temperature, the larger entropy must outweigh the lower stability of the pretzel structure. The Nose-Hoover simulations contain the information about the heat uptake, and hence the entropy ass0ciated with the atomic degrees of freedom (structural, vibrational and rotational entropy). A compariaon between the entropy of a fullerene and a linear chain (with equal numbers of atoms) indicates a nearly constant entropy difference 1>.8 "" 2kB (per atom) between these structures [34]. The binding energy difference (per atom) between a fullerene and a chain of ",,1 eV leads, together with the

they are reproducible, can be viewed as a signature of a phase transition which, rigorously speaking, should only occur in an infinite system. Even though the "phase transitions" are gradual in finite systems, the concept of

"phll8es", separated by reproducible features in the specific hea.t, appea.cs to be useful.

Perbaps the most straight-forward characterization of these "phases" can be achieved by capturing the atomic motion on a. video movie, or at leaat by visualizing "snap sho1o" of the MD simulation, as shown in Fig. 2. Fig.2(a) shows that the C 60 molecule keeps its structure at least up to T = I, 000 K. After the first "phase transition" just below T = 3, 000 K, the systems gets ''floppy'', as shown in Fig. 2(b). At times, C-C bonds break open in

above value for the entropy difference, to an estimated "melting temperatureU of fuHerelles lleM 5,800 K. Thi~ value is of the same order of magnitude CIo!'J the value obtained in the MD simulation, and also close to the melting point of graphite, TM (graphite) = 3,823 K [35]. These results confirm that the "melting traDBition" in fuHerenes at TM "" 4,000 K is driven mainly by the vibrational and

structural entropy.

this "phase" , and rings of carbon atoma open like a valve. Such processes are always reversible; all a.toms "know"

their equilibrium positions. Beyond the "melting temperature" of T M s::::l 4, 000 K, the system transforms to a "pretzel" consisting of linked rings, as shown in Fig. 2(e). Experimental evidence for such a transition has recently

been obtained from diffusion experimen10 [32,33]. At a temperature exceeding 5,000 K, the rings break open,

IV. SUMMARY AND CONCLUSIONS I have discussed successful application of both ab initio and parametrized techniques to quantitative calculations of the stability and electronic properties of carbon clusters, in particular carbon fullerenes and related systems. Theoretical resul10 indicate that

yielding a structure composed of linked chains, shown in

Fig. 2(d). As shown in Figs. 2(e) and (f), the continuous structure of this aggregate eventually breaks into smaller fragments. From this point aD, the simulations describe a

system of chain and ring fragmen10 rather than the thermodynamics of C so . More meaningful for the characterization of the different "phases" than mere visualization of "snap shots" is

the (time-averaged) binding energy distribution in the system, based on the energy decomposition of Eq. (2). This appears to be more meaningful than a discussion of changing coordination numbers which are ill-defined in amorphous systems.

Below the "melting temperature" TM "" 4,000 K, all atoms are essentially equivalent and their binding energy is characterized by a single peak in the distribution near 7 eV. This peak broadens and shifts to lower values with increasing temperature. In the "pretzel phase", the binding energy distribution changes drastically to a bi-modal distribution which describes the occurrence of two inequivalent types of sites: the twofold coordinated atoms in the strained rings and the more stable multiply-coordinated atoms at the links of these rings. The onset of the "linked chains phase" is marked by a third peak near a binding energy of "" 5 eV associated with chain ends. At even

• At T = 0, the equilibrium shapes offree C n clusters are chains and rings for n < 20, spherical fuHerene cages for n > 20, and multi-walled onions for n > 700 atoms. Entropy is expected to playa significant role at T> O. • The optical response of fullerenes is dominated by collective excitations at 1iw.",,6 eV and Iiw q ""20 eV with counterparts in the .. and (f plasmons of graphite.

• Superconductivity in the alkali doped C60 solid can be explained by the standard BCS theory. The important factors responsible for a large critical temperature T c are a. large electronic deIl5ity of states

at EF and efficient coupling of conduction electrons by .tiff on-ball modes. • The threshold for inelastic C2 • 0-C60 collision.• is at E CM "" 200 eV. The smaller cluster "melts" upon impact.

• Upon heating, free fullerenes show a structural transformation to ''pretzels'' at T "" 4, 000 K, which is driven by vibrational and structural entropy.

-S616-

Journal of the Korean Physical. Society(proc. Suppl.), Vol. 28, December 1995

ACKNOWLEDGEMENT This work has been performed in collaboration with (alphabetically) George Bertsch, Aurel Bulgac, Richard Enbody, Seong Gon Kim, Michael Schliiter, Yang Wang, and Weiqing Zhong, whose contributions are gratefully acknowledged. Financial support has been provided by the National Science Foundation under Grant No. PRY8920927, the Air Force Office of Scientific Research under Grant No. F4962Q-92-J-0523DEF, and by the sponsors of the 1995 conference in Taejon, Korea.

REFERENCES

[1] H. W. Kroto, J. R. Heath, S. C. O'Brien, R. F. Curl, and R. E. Smalley, Nature 318, 162 (1985). [2] W. Kriitschmer, L. D. Lamb, K. Fostiropoulos, and D. R. Hullman, Nature 347, 354 (1990). [3] A. F. Hebard, M. J. Rosseinsky, R. C. Haddon, D. W. Murphy, S. H. Glarum, T. T. M. Palstra, A. P. Ramirez, and A. R. Kortan, Nature 350, 600 (1991). [4] M. J. Rosseinsky, A, P. Clarum, D. W. Murphy, R. C. Haddon, A. F. Hebard, T. T. M. Palstra, A. R. Kortan, S. M. Zalmrak, and A. V. Makhija, Phys. Rev. Lett. 66, 2830 (1991). [5] Daniel Ugarte, Nature 359, 707 (1992). [6] Snmin Iijima, Nature 354,56 (1991); Snmio lijima, Toshinari lebihashi, and Yoshinori Ando, Nature 356, 776 (1992). [7] J. R. Heath, S. C. O'Brien, Q. Zhang, Y. Liu, R. F. Curl, H. W. Kroto, and R. E. Smalley, J. Am. Chem. Soc. 107, 7779 (1985), [8] P. Hohenherg and W. Kohn, Phys. Rev. 136, B864 (1964); W. Kohn and 1. J. Sham, Phys. Rev. 140, A1ll3 (1965). [9J D. Tomanek and Michael A. Schluter, Phys. Rev. Lett. 67, 2331 (1991). [10] W. Zhong, D. Tomanek and George F. Bertscil, Solid State Common. 66, 607 (1993). [11] J. C. Slater and G. F. Kuster, Phys. Rev. 94, 1498 (1954). [12] W. G. Hoover, Phys. Rev, A31, 1695 (1985); S Nose, Mol. Phys. 52, 255 (1984). [13J M. P. Allen and D. J. Tildewey, Computer Simulation of Liquids (Oxford, New York, 1990). [14] Synthesis and topology of large fullerenes has been reviewed by Robert F. Curl and Richard E. Smalley in Scientific American, October 1991, p. 54. [15] D. Tomanek, W. Zhong, and E. Krastev, Phys. Rev. B48, 15461 (1993).

[16] G. F. Bertsch, A. Bulgac, D. Tomanek and Y. Wang, Phys. Rev. Lett. 67, 2690 (1991). [17] G. D. Mahan, Many-Particle Physics, (Plenwn Press, New York, 1981). [18] S""wnu Saito and At.""hi O.hiyama, Phys. Rev. Lett. 66,2637 (1991), [19] H. Ajie, M. M. Alvarez, S. J. Anz, R. D. Beck, F. Diederich, K. Fostiropoulos, D. R. Huffman, W. Kratschmer, Y. Rubin, K. R Sc-.hriver, D. Sensharma, and R. L. Whetten, J. Phys. Chem. 94,8630 (1990). [20] I. V. Hertel. H. Steger, J. de Vries, B. Weisser, C. Menzel, B. Kamke and W. Kamke, Phys. Rev. Lett. 68, 784 (1992). [21] J. H. Weaver, J, L. Martins, T. Komeda, Y. Chen, T. R. Ohno, G. H. Kroll, N. Thoullier, R. E. Haulier and R. E. Smalley, Phys. Rev. Lett. 66, 1741 (1991). [22] Yahachi Saito, Hisanori Shinohara, and Akinori Obshita, Japan. J. Appl. Phys. 30, LlO68 (1991); G. Gensterblum, J. J. Pireaux, P. Thiry, R. Caudano, J. P. Vigneron, Ph. Lambin, A. A. Lucas and W. Kratschmer, Phys. Rev. Lett. 67, 2171 (1991). [23] G. Gensterblwn, J. J. Pireaux, P. Thiry, R. Caudano, J. P. Vigneron, P. Lambin and A. A, Lucas, Phys. Rey. Lett. 67, 2171 (1991). [24] A. Bulgac and N. Ju, Phys. Rev. B46, 4297 (1992); Nengjiu Ju, Aurel Bulgac and John W. Keller, Phys. Rev. B48,9071 (1993). [25J K. Zeppenield, Z. Phys. 211,391 (1968); K. Zeppenfeld, Z. Phys. 243, 229 (1971); H. H. Venduws, Phys. Stat. Sol. (b) 71, 609 (1975); R. Klucker, M. Skibowski and W. Steinmann, ibid, 65, 703 (1974); U. Buchner, ibid, 81, 227 (1977); U. Diebold, A. Preisinger, P. Schattsdchneider and P. Varga, Surf. Sci. 197,430 (1988). [26J M. Schluter, M. Lannoo, M. Needels, G. A. BaraIf, and D. Tomanek, Phys. Rev. Lett. 68, 526 (1992). [27] W. L. McMillan, Phys. Rev. 167,331 (1968). [28] M. Schliiter, M. Lannoo, M. Needels, G. A. BaraIf, and D. Tomanek, J. Phys. Chem. Solids 53, 1473 (1992). [29] M. Lannoo, G. A. B.,.aIf, M. Schluter, and D. Tomanek, Phys. Rev. B44, 12106 (1991). [30J Seong Goo Kim and David Tomanek, Phy.. Rev. Lett. 72, 2418 (1994). [31] Ennja Kim, Young Hee Lee and Joe Young Lee, Phys. Rev. B48, 18230 (1993). [32] J. M. Honter, J. L. Fye, E. J. Roskamp, M. F. Jarrold, J. Phys. Chem. 98, 1810 (1994). [33] G. von Heiden, N. Gotts, and M. T. Bowers, Nature 363, 60 (1993). [34] This is true below the "melting point"; both structures are very similar and hence have the same entropy above the "melting point". [35] eRC Handbook of Chemi.try and Physics, 62th edition (CRC Press, Boca Raton, Florida, 1990) p. B-1O.

Building a Better World with Buckyballs David TOMANEK Department of Phy&ic& and A.dronomy and Center for Fundamental Materials RC8eorch Michigan State Univcrsity, Ecut Lan8'ng, Michigan 48894-1116, U. S. A.

The 0 60

"buckyball" a prominent member of the recently discovered family of fullerene molecules, I

is an unusual system with exciting properties. This contribution summarizes the present state of theoretical understanding of the equilibrium structure of carbon clusters, in particular the fullerenes,

the optical properties of individual fullerene molecules, superconductivity in the alkali-intercalated Ceo solid, and the disintegration of fullerenes in collisions and at high temperatures.

I. INTRODUCTION Until very recently, the only stable bulk forms of elemental carbon have been believed to be graphite and diamond. About ten years ago, this conventional wisdom has been challenged by the discovery of the stable C60 molecule with a spherical hollow cage [1]. This molecule, .tKJmetimes called "buckyball", turned out to be only a particular representative of the family of ''fullerene" molecules, named so for their close resembla.ncc to the geodesic dome structures created by the architect Buckminster Fuller. Later on, it has been found that Cso molecules can aggregate to form a molecular crystal. The interest in C60 rose dramatically following the successful development of a mass production technique for this system [2]. The resulting research first concentrated on characterizing this molecule and the corresponding solid. Next, spurred by the discovery of superconductivity in the alkali intercalated C so solid [3,4], substantial effort has been invested in modifying the C 60 molecule and solid, and in the synthesis of other fullerenes. Ongoing research focuses both on the structural and electronic properties of C60inspired carbon fullerenes. At present, most emphasis is pla 20, we find rings to be more favorable than chains, since releasing the dangling bond energy of a chain easily offsets the bending energy when forming a ring. At these 181'ger ai~es, however, higher coordinated structures turn out to be energetically much more favorable. For n > 20, we find the hollow fullerenes to be the most stable isomers. Alec in this size range, the average binding energy per atom is gradually increasing with in-

creasing fullerene size, approaching the value found in a graphene sheet [15]. At sizes exceeding 700 atoms, finally, multi-walled structures are found to be most stable, due to the significance of the attractive interaction between adjacent walla [15]. The Coo does not appear to be exceptionally stable. Since in thermodynamic equilibrium the relative abundance of different cluaters should reflect their stability, our

0.7 ~

:> OJ

~

'" 0 0

i'il

6.6

...... ' ...

6.5

.x'

,"

~..

" .•.•.•.••........ •...... "/.:.~.,, .....

6.4 6.3 6.2

6.1 6. a

.........

"

,

..jIIl

"

••-"'..~_...L'_-'-_L-~_--'-_--'-..--.J

~

~

~

M

~

~

50

9

60

n

Fig. 1. Binding energy per atom E coo in small carbon eluate... as a function of eluster size n, (a) for n ~ 20 and (b) for n ~ 20. R..aults for cbains (0) are connected by a solid line, results for ~ (0) are connected by a dashed line, and results for planar grapbite flakes (.) are connected by a dotted line. Results for buckled fullerene caps with a pentagonal ( x) or a hexagonal baais (+) are connected by a dashed line. Results for hollow fullerene cages (.) are connected by a solid line. (From Ref. [9], @American Physical Society.)

results would suggest a continuous size distribution of carbon fullerenes in the mass spectra. This is in clear con-

2. Collective electronic excitations in Ceo clusters

trast with the observed abundance of the 60-atom struc-

The structural similarity between a Coo molecule and graphite raises the question, whether the optical response of this finite system may have any resemblance with that of macrOBCopic graphite. In the following, I willleview resulta for the dynamical dipole response of flee Coo me>-

ture. We must conclude that simulations beyond these T '" 0 stability considerations are nece..ary to explain

the abundance of the "magic" Coo cluster in the m.... spectra.

Journal of the Korean Physical Society(Proc. SuppI.), Vol. 28, December 1995

-8612-

leeules, published previously in Ref. [16], with emphasis on the discussion of collective plasmon-like excitations. The optical response of clusters to an external field is described within linear response using the Random Phase Approximation (RPA) [17]. In the present case, the single-particle spectrum is obtained using the parametrized LCAO Hamiltonian discussed previously. The occupied states spread over 19.1 eV, in good agreement with the publisbed LOA value of 18.8 eV [18J. The calculated gap between the highest occupied molecular orbital (HOMO) and the lowest unoccupied molecular orbital (LUMO) is 2.2 eV, larger than the 1.8 eV value which is underestimated in LDA [18]. The "1r" states near the HOMO-LUMO gap, and the more strongly bound "IT" states have a similar character as the corresponding states in graphite. The icosahedral symmetry of Cso allows us to distinguish singly-, triply-, quadruply- and pentuply-degenerate levels. A large number of optical transitions is allowed by the dipole selection rules. In the particular case of a dynamical dipole field along the z-direction, which is applied to a spherical molecule such as Cs o, the calculation can be simplified significantly by anticipating the form of the dipole operator which describes the response of the system. As discussed in Ref. [9], the dipole operator D, is dominated by two contributions:

Dl1)

J

origina.ting in the intersite charge trans--

fer across the molecule, and D}2) , stemming from the polarization of individual carbon atoms. In the free response, which ignores the screening of transitions by electron-hole pair excita.tions, the lowest dipole-allowed tr8Illlition is the IIOMO - t LU MO + I transition which occurs at an energy 1u..J < 3 eV. In the RPA treatment of dynamical screening, the low-lying transitions are slightly blue shifted and, more important, their oscillator strength is reduced by a factor of typically 10 with respect to the free response. A factor of 400 quenches the HOMO - t LU MO + I transition to only an insignificant peak in the spectrum. Even though the calculated spectrum in the frequency range rn" < 10 eV resembles the observed absorption spectrum in a dilute Cso solution [19), the integrated oscillator strength in this range remains well below the value of 240 (which is the total number of active electrons), as predicted by the fsum rnle. The missing oscillator strength is fOWld at higher energies. The oscillator strength, which occurs as a dense featureless spectrum in the free response, piles up to a giant collective excitation at rn" "" 30 eV in the RPA response calculated with ill') only. The consideration of also Dlztinduced transitions causes a fragmentation and red shift of this mode into an energy range of rn" "" 20 eV. This prediction has been subsequently confirmed by the observation of a giant resonance at rn" '" 20 eV in the photoionization spectrnm of CGO [20]. Collective excitations at frequencies ranging between 20 - 30 eV have also been observed in Cso films [21-23). To investigate the nature of this collective mode, an

LOA-RPA calculation was performed for an infinitely thin spherical jellium shell with the radius of Cso, carrying 240 conduction electrons [16]. The calculation predicted a single absorption peak at a frequency &.1,,;15 - 20 eV, which lies very close to the Mie plasmon frequency rn"Mi, = h[41rpe 2/(3m»)'/2 ",25 eV of a solid metal sphere with 240 free electrons and the radius of the Cs o cluster. The origin of the high value of the collective mode frequency is consequently the large valence electron density p in the CGO molecule. This leads to the conclusion that collective electronic excitations occur in fullerenes as small as tbe C so molecule. The nature of these modes, which occur at frequencies far beyond the HOMO-LUMO gap, resembles closely that of a classical Mie plasmon. A more refined calculation of the RPA response of fullerenes to external fields [24], not restricted to the dipole response described by D}') and Di2 ) , shows that the excitation spectrum of probably all fullerenes (investigated were C,o, C so and 070) is dominated by the above discussed "(1" mode at hw.,.R::20 eV and a softer "1f'" mode at rn"."'6 eV. These two modes have also been observed in electron energy loss spectra of Cs o fullerite films [23], and appear to be the analogues of the 1r and IT plasmons in graphite [25]. In graphite, the low-frequency 1r mode has been interpreted by the in-plane response of the weakly bound P. system to a field parallel to the layers. The high-frequency IT mode has been assigned to the out-ofplane motion of the strongly bound IT system of 8 and P electrons in response to a field perpendicular to the layel'S.

It appears that the finite fullerene molecules show a well-defined signature of plasmon modes which are closely related - in nature and in frequency - to the IT- and 1rplasmons of graphite. The large oscillator strength of these modes is collected from lower-lying particle-hole excitations which consequently experience strong dynamical screening.

3. Superconductivity in the alkali doped CGO solid Potentially the most important property of the C so solid is its superconducting behavior when doped with alkali atoms [3,4). In the following, I will present a quantitative Bardeen-Cooper-8chrieffer (BC8) theory which has been used successfully to describe the superconducting behavior of Cso [26]. The electronic states of the alkali doped M,C GO solid are calculated using the LOA and the LCAO formalism discussed above. The vibr.... tional modes of the solid are determined using an extended Keating Hamiltonian which describes both on-ball and inter-ball vibrations. McMillan's expression for the critical temperature for superconductivity Tc reads [27] Tc

_ rn,,'og -

(-1.04(1+ .\) ) 1.2 kB ezp .A - ,,- _ 0.62.\,,-

(9)

Building a Better World with Buckyballs - David TOMANEK In accordance with other standard superconductors, 1" "" 0.1 was used for the effective Coulomb repulsion. The stiff on-ball vibrational modes of Coo yield .~' •• "" 1400 K for the "Debye temperature" of the solid. ir.'th the electronphonon coupling constant A "" 0.6, to be derived below, we can explain the observed value T, "" 30 K in Rb3 C. O

[4]. The electron-phonon coupling constant is given by A = 2N(Ep )V, where N(E p ) is the electronic density of states at the Fermi level, and Y is the Bardeen-Pines interaction which couples two electrons to a Cooper pair. The large value of A is a consequence of both a large density of states at the Fermi level and a strong coupling of these states to vibrational states. The conduction band is derived from the lowest unoccupied molecular orbital (LUMO) of C. O, and has P. character. Due to the small inter-ball hopping, the width of this band is small, W""0.5 eV [18,28J. For a featureless (e.g. rectangular) band, one can estimate N(Ep ) "" 6/0.5 ey-l .. 10 ey-l. LDA calculations give N(Ep ) "" 20 ey- 1 for a half filled band [18,28]. This density of states is at least one order of magnitude larger than that of intercalated graphite, consistent with the finding that T,(intercalated graphite) «Tc(M3Cso), The vibrational eigenmodes of the crystal were determined using an extended Keating Hamiltonian, with parameters adjusted to reproduce the vibrational spectra of the C.O solid. The coupling to the conduction states was investigated for each of these modes. These calculations showed that coupling of the librational modes at v "" 10 em-I can be neglected, while inter-ball optical modes at v .. 100 em-I couple weakly. The important modes are on-ball modes at a frequency range v "" 200 - 1600 em-I. Among the most strongly coupling modes are the radial buckling H. modes at v" 400 em -1, the tangential pentagon breathing A. mode at v "" 1600 em-I. and tangential optical H. modes at V"" 1600 em-I. These modes gave a value of V",,21 meV per Cso. The above determined large values of V and of N(E p ) are responsible for a large electronphonon coupling constant A. The dominant contribution of on-ball modes to the electron-phonon coupling makes it possible to treat electron-phonon coupling in relationship to a dynamical Jahn-Teller effect for the charged C. o molecule, and consider solid Cso as a molecular crystal [29]. In this case, when changing the alkali intercalant M in M3CSO, Aand consequently also T, should only depend on the Cso-C.o separation which modifies N (EF). One would expect an increase of T" with increasing lattice constant of M3C.o, which is achieved by substituting a heavier alkali element M [28]. The same argument would lead to the conclusion that a reduction of the lattice constant, due to increasing pressure, should result in a reduction of T,. Both these effects have been verified experimentally [28]. In conclusion, standard BCS theory was found to be capable of providing a quantitative explanation of super-

I,.

-5613-

conductivity in the alkali doped Cso solid. The observed large value of T, is linked to the high Debye temperature, a large value of N(E p ), and a strong coupling of on-ball vibrational modes to states at Ep [26,28]. 4.

Collision dynamics of fullerenes

Next, I will discuss the stability and reactivity of C n fullerene clusters in binary collisions. Of particular interest in this study was the question of a potential synthesis of more complex structures, such as multi-walled fullerenes (or "bucky onions") [5], by impact-induced encapsulation of the smaller C. o buckyball inside the larger C240 fullerene. In order to better understand the reaction dynamics, the motion of the individual atoms during the collision process was visualized in

& video

movie.

Microcanonical molecular dynamics simulations of the collision process were performed at different initial center-of-m.... kinetic energies. The Cso and the C240 clusters were prepared in their equilibrium structures. In the first set of simulati()ns investigating central collisions, the clusters were given an initial linear momentwn, zero angular momentum, and the impact parameter was set to zero.

At a low 10 eV center-of-m.... kinetic energy, the collision between the C240 and the C.o clusters could be best characterized as an elastic recoil. At a ten times higher center-of-mass energy of 100 eV, the C,.o-C. o collision is best described as quasielastic scattering. At the point of impact of C.O onto the C 24 0 cluster, one can observe a heat- and shock-wave propagating fast within the structure, starting at the point of contact. The C,.o-C. o agglomerate is capable of storing the large surplus energy in a substantial structural deformation and the many vibrational degrees of freedom of the system. In spite of the extreme deformations which even result in a negative Gaussian curvature of the

C240

cluster, both clusters depart intact, without exchanging any atoms. Finally, at only three times higher center-of-m.... energy of 300 eV, the C,.o-C.o collision leads to an impactinduced fragmentation. The intuitive expectation, that the more rigid C60 structure might penetrate the "floppy" wall of the larger C240 fullerene, proves to be incorrect. The opposite process occurs - it is the smaller C60 cluster which fragments first, leaving the larger C240 structure vibrationally highly excited, yet intact. Cso is observed to fragment into a structure consisting of linked chains and rings, as well as fragments. A very similar fragmentation dynamics is also observed in simulations asswning

&

nonzero impact parameter and nonzero ini-

tial angular momentum of the fullerenes prior to collision. The physics underlying this particular fragmentation process is relatively simple. Upon impact, the exces&ive center-of-mass kinetic energy is distributed into the internal degrees of freedom of both clusters; this vibra-

-8614-

Journal of the Korean Physical Society(Pmc. Suppl.), Vol. 28, December 1995

(a) Solid phase

(b) Floppy phase

(e) Pretzel phase

T=1000

T=3000 K

T=4200 K

(d) Linked chains

(f) Chain gas

T=5000 K

T=10200 K

cf)

Fig. 2. llSnap shots" illustrating the geometry of a 060 dU8teT at temperatures COI'1"'""Ip'l to the different "phases"

dillCWlOed in the text. (From Ref. [30], @American Physical Society.) tional energy appears as heat. The fewer degrees of freedom of the smaller C.o cluster experience a higher excitation which results in a higher temperature. Due to the limited amount of vibrational energy which can be stored in the anharmonic potentials, the energy surplus is consumed in the heat of "melting" and partly the heat of "evaporation". The structural transformation of the fragmented Ceo cluster at high temperatures is driven by the vibrational and structural entropy which is obviously much higher for the floppy one-dimensional chain and ring substructures than the more rigid fullerene structure. If this explanation is correct~ the same structure con~ sisting of linked rings and chains should also occur in isolated fullerenes which have been exposed to temperatures beyond those causing melting. AJ, will be shown in the following Subsection, this is indeed the case. More important, this establishes an intriguing link between the impact- and thermally-induced fragmentation of clusters.

Ii.

How do buckyballs melt?

The present study, originally inspired by the surprising results of above described inelastic collisions, is intended to answer some fundamental questions related to the nature of thermally induced structural transformations in fullerenes and finite clusters in general. The first important question is, whether atomic clusters - such as fullerenes - undergo "phase transitions" such as melting, and what the "phase diagram" would look like. Next, one would like to know how to best characterize the.. "phases". Finally, one would like to understand the drivang force for such "phase transitions" . These and some other related questions have been addressed in a Nose-Hoover molecular dynamics simula.tion of the melting and evaporation process of three prototype fullerenes, namely C20, Coo, and C 240 . The detaila of the simulation are discussed in Ref. [30]. The reBults

Building a Better World with Buckyballa - David TOMANEK

-S615-

presented below complement nicely those of recent microcanonical ensemble simulations on C 60 and C70 [31]. The key result of the simulation is the total energy of an iaolated fullerene as a function of heat hath temperature. In the temperature range of interest, namely between 1,000 K and 10,000 K, the energy E shows a generally linear increase with temperature. The specific heat cv = dE/ dT is generally close to the classical value cv = 3kB/particle. Strong peaks in the specific heat occur close to 3,000 K and 4,000 K. The peaks get more pronounced with increasing size of the system and, since

higher temperatures, the spectrum broadens and the average stability of the structure decreases. A simple estimate of the "melting transition" from fullerenes to pretzels can be obtained by comparing the free energies of the two structures which must be equal at the melting point. At this temperature, the larger entropy must outweigh the lower stability of the pretzel structure. The Nose-Hoover simulations contain the information about the heat uptake, and hence the entropy ass0ciated with the atomic degrees of freedom (structural, vibrational and rotational entropy). A compariaon between the entropy of a fullerene and a linear chain (with equal numbers of atoms) indicates a nearly constant entropy difference 1>.8 "" 2kB (per atom) between these structures [34]. The binding energy difference (per atom) between a fullerene and a chain of ",,1 eV leads, together with the

they are reproducible, can be viewed as a signature of a phase transition which, rigorously speaking, should only occur in an infinite system. Even though the "phase transitions" are gradual in finite systems, the concept of

"phll8es", separated by reproducible features in the specific hea.t, appea.cs to be useful.

Perbaps the most straight-forward characterization of these "phases" can be achieved by capturing the atomic motion on a. video movie, or at leaat by visualizing "snap sho1o" of the MD simulation, as shown in Fig. 2. Fig.2(a) shows that the C 60 molecule keeps its structure at least up to T = I, 000 K. After the first "phase transition" just below T = 3, 000 K, the systems gets ''floppy'', as shown in Fig. 2(b). At times, C-C bonds break open in

above value for the entropy difference, to an estimated "melting temperatureU of fuHerelles lleM 5,800 K. Thi~ value is of the same order of magnitude CIo!'J the value obtained in the MD simulation, and also close to the melting point of graphite, TM (graphite) = 3,823 K [35]. These results confirm that the "melting traDBition" in fuHerenes at TM "" 4,000 K is driven mainly by the vibrational and

structural entropy.

this "phase" , and rings of carbon atoma open like a valve. Such processes are always reversible; all a.toms "know"

their equilibrium positions. Beyond the "melting temperature" of T M s::::l 4, 000 K, the system transforms to a "pretzel" consisting of linked rings, as shown in Fig. 2(e). Experimental evidence for such a transition has recently

been obtained from diffusion experimen10 [32,33]. At a temperature exceeding 5,000 K, the rings break open,

IV. SUMMARY AND CONCLUSIONS I have discussed successful application of both ab initio and parametrized techniques to quantitative calculations of the stability and electronic properties of carbon clusters, in particular carbon fullerenes and related systems. Theoretical resul10 indicate that

yielding a structure composed of linked chains, shown in

Fig. 2(d). As shown in Figs. 2(e) and (f), the continuous structure of this aggregate eventually breaks into smaller fragments. From this point aD, the simulations describe a

system of chain and ring fragmen10 rather than the thermodynamics of C so . More meaningful for the characterization of the different "phases" than mere visualization of "snap shots" is

the (time-averaged) binding energy distribution in the system, based on the energy decomposition of Eq. (2). This appears to be more meaningful than a discussion of changing coordination numbers which are ill-defined in amorphous systems.

Below the "melting temperature" TM "" 4,000 K, all atoms are essentially equivalent and their binding energy is characterized by a single peak in the distribution near 7 eV. This peak broadens and shifts to lower values with increasing temperature. In the "pretzel phase", the binding energy distribution changes drastically to a bi-modal distribution which describes the occurrence of two inequivalent types of sites: the twofold coordinated atoms in the strained rings and the more stable multiply-coordinated atoms at the links of these rings. The onset of the "linked chains phase" is marked by a third peak near a binding energy of "" 5 eV associated with chain ends. At even

• At T = 0, the equilibrium shapes offree C n clusters are chains and rings for n < 20, spherical fuHerene cages for n > 20, and multi-walled onions for n > 700 atoms. Entropy is expected to playa significant role at T> O. • The optical response of fullerenes is dominated by collective excitations at 1iw.",,6 eV and Iiw q ""20 eV with counterparts in the .. and (f plasmons of graphite.

• Superconductivity in the alkali doped C60 solid can be explained by the standard BCS theory. The important factors responsible for a large critical temperature T c are a. large electronic deIl5ity of states

at EF and efficient coupling of conduction electrons by .tiff on-ball modes. • The threshold for inelastic C2 • 0-C60 collision.• is at E CM "" 200 eV. The smaller cluster "melts" upon impact.

• Upon heating, free fullerenes show a structural transformation to ''pretzels'' at T "" 4, 000 K, which is driven by vibrational and structural entropy.

-S616-

Journal of the Korean Physical. Society(proc. Suppl.), Vol. 28, December 1995

ACKNOWLEDGEMENT This work has been performed in collaboration with (alphabetically) George Bertsch, Aurel Bulgac, Richard Enbody, Seong Gon Kim, Michael Schliiter, Yang Wang, and Weiqing Zhong, whose contributions are gratefully acknowledged. Financial support has been provided by the National Science Foundation under Grant No. PRY8920927, the Air Force Office of Scientific Research under Grant No. F4962Q-92-J-0523DEF, and by the sponsors of the 1995 conference in Taejon, Korea.

REFERENCES

[1] H. W. Kroto, J. R. Heath, S. C. O'Brien, R. F. Curl, and R. E. Smalley, Nature 318, 162 (1985). [2] W. Kriitschmer, L. D. Lamb, K. Fostiropoulos, and D. R. Hullman, Nature 347, 354 (1990). [3] A. F. Hebard, M. J. Rosseinsky, R. C. Haddon, D. W. Murphy, S. H. Glarum, T. T. M. Palstra, A. P. Ramirez, and A. R. Kortan, Nature 350, 600 (1991). [4] M. J. Rosseinsky, A, P. Clarum, D. W. Murphy, R. C. Haddon, A. F. Hebard, T. T. M. Palstra, A. R. Kortan, S. M. Zalmrak, and A. V. Makhija, Phys. Rev. Lett. 66, 2830 (1991). [5] Daniel Ugarte, Nature 359, 707 (1992). [6] Snmin Iijima, Nature 354,56 (1991); Snmio lijima, Toshinari lebihashi, and Yoshinori Ando, Nature 356, 776 (1992). [7] J. R. Heath, S. C. O'Brien, Q. Zhang, Y. Liu, R. F. Curl, H. W. Kroto, and R. E. Smalley, J. Am. Chem. Soc. 107, 7779 (1985), [8] P. Hohenherg and W. Kohn, Phys. Rev. 136, B864 (1964); W. Kohn and 1. J. Sham, Phys. Rev. 140, A1ll3 (1965). [9J D. Tomanek and Michael A. Schluter, Phys. Rev. Lett. 67, 2331 (1991). [10] W. Zhong, D. Tomanek and George F. Bertscil, Solid State Common. 66, 607 (1993). [11] J. C. Slater and G. F. Kuster, Phys. Rev. 94, 1498 (1954). [12] W. G. Hoover, Phys. Rev, A31, 1695 (1985); S Nose, Mol. Phys. 52, 255 (1984). [13J M. P. Allen and D. J. Tildewey, Computer Simulation of Liquids (Oxford, New York, 1990). [14] Synthesis and topology of large fullerenes has been reviewed by Robert F. Curl and Richard E. Smalley in Scientific American, October 1991, p. 54. [15] D. Tomanek, W. Zhong, and E. Krastev, Phys. Rev. B48, 15461 (1993).

[16] G. F. Bertsch, A. Bulgac, D. Tomanek and Y. Wang, Phys. Rev. Lett. 67, 2690 (1991). [17] G. D. Mahan, Many-Particle Physics, (Plenwn Press, New York, 1981). [18] S""wnu Saito and At.""hi O.hiyama, Phys. Rev. Lett. 66,2637 (1991), [19] H. Ajie, M. M. Alvarez, S. J. Anz, R. D. Beck, F. Diederich, K. Fostiropoulos, D. R. Huffman, W. Kratschmer, Y. Rubin, K. R Sc-.hriver, D. Sensharma, and R. L. Whetten, J. Phys. Chem. 94,8630 (1990). [20] I. V. Hertel. H. Steger, J. de Vries, B. Weisser, C. Menzel, B. Kamke and W. Kamke, Phys. Rev. Lett. 68, 784 (1992). [21] J. H. Weaver, J, L. Martins, T. Komeda, Y. Chen, T. R. Ohno, G. H. Kroll, N. Thoullier, R. E. Haulier and R. E. Smalley, Phys. Rev. Lett. 66, 1741 (1991). [22] Yahachi Saito, Hisanori Shinohara, and Akinori Obshita, Japan. J. Appl. Phys. 30, LlO68 (1991); G. Gensterblum, J. J. Pireaux, P. Thiry, R. Caudano, J. P. Vigneron, Ph. Lambin, A. A. Lucas and W. Kratschmer, Phys. Rev. Lett. 67, 2171 (1991). [23] G. Gensterblwn, J. J. Pireaux, P. Thiry, R. Caudano, J. P. Vigneron, P. Lambin and A. A, Lucas, Phys. Rey. Lett. 67, 2171 (1991). [24] A. Bulgac and N. Ju, Phys. Rev. B46, 4297 (1992); Nengjiu Ju, Aurel Bulgac and John W. Keller, Phys. Rev. B48,9071 (1993). [25J K. Zeppenield, Z. Phys. 211,391 (1968); K. Zeppenfeld, Z. Phys. 243, 229 (1971); H. H. Venduws, Phys. Stat. Sol. (b) 71, 609 (1975); R. Klucker, M. Skibowski and W. Steinmann, ibid, 65, 703 (1974); U. Buchner, ibid, 81, 227 (1977); U. Diebold, A. Preisinger, P. Schattsdchneider and P. Varga, Surf. Sci. 197,430 (1988). [26J M. Schluter, M. Lannoo, M. Needels, G. A. BaraIf, and D. Tomanek, Phys. Rev. Lett. 68, 526 (1992). [27] W. L. McMillan, Phys. Rev. 167,331 (1968). [28] M. Schliiter, M. Lannoo, M. Needels, G. A. BaraIf, and D. Tomanek, J. Phys. Chem. Solids 53, 1473 (1992). [29] M. Lannoo, G. A. B.,.aIf, M. Schluter, and D. Tomanek, Phys. Rev. B44, 12106 (1991). [30J Seong Goo Kim and David Tomanek, Phy.. Rev. Lett. 72, 2418 (1994). [31] Ennja Kim, Young Hee Lee and Joe Young Lee, Phys. Rev. B48, 18230 (1993). [32] J. M. Honter, J. L. Fye, E. J. Roskamp, M. F. Jarrold, J. Phys. Chem. 98, 1810 (1994). [33] G. von Heiden, N. Gotts, and M. T. Bowers, Nature 363, 60 (1993). [34] This is true below the "melting point"; both structures are very similar and hence have the same entropy above the "melting point". [35] eRC Handbook of Chemi.try and Physics, 62th edition (CRC Press, Boca Raton, Florida, 1990) p. B-1O.